Has a body-centred cubic (BCC) crystal structure. It is soft and ductile and imparts these properties to the steel. Very little carbon (less than 0.01% carbon will dissolve in ferrite at room temperature). Often known as iron.
This is the structure of iron at high temperatures (over 912 deg C).
Has a face-centre cubic (FCC) crystal structure. This material is important in that it is the structure from which other structures are formed when the material cools from elevated temperatures. Often known as iron. Not present at room temperatures.
A laminated structure formed of alternate layers of ferrite and cementite.
It combines the hardness and strength of cementite with the ductility of ferrite and is the key to the wide range of the properties of steels. The laminar structure also acts as a barrier to crack movement as in composites. This gives it toughness.
As carbon content increases beyond 0.8%, no more pearlite can be formed.
The excess carbon forms cementite which is deposited in between the pearlite grains. This increases the hardness, but slightly reduces the strength. The ductility of all plain carbon steels over 0.8% carbon is very low.
Properties of Carbon Steels Bars and forgings for a wide range of engineering components. Connecting rods, springs, hammers, axle shafts requiring strength and toughness. Very strong, heat treatable to produce a wide range of properties in quenched and tempered conditions. Difficult to weld. Can become brittle below room temperature. 0.25 - 0.6 General engineering uses for a mild steel Strong, ductile, no useful hardening by heat treatment except by normalizing, but can be work-hardened. Weldable. Ductile-brittle transition temperature is just below room temperature 0.1 - 0.25 Pressings where high formability required Soft, ductile, no useful hardening by heat treatment except by normalizing, but can be work-hardened. Weldable. 0.01 - 0.1 Applications Properties Carbon content wt %
Properties of Carbon Steels Cutting tools like wood chisels, files, saw blades . Wear resistant and can be made very hard at expense of toughness and ductility. Cannot be welded. Tend to be brittle if the structure is not carefully controlled 0.9 - 2.0 Used where maximum strength rather than toughness is important. Tools, wear resisting components ( piano wire and silver steels are in this group). Strong, whether heat treated or not. Ductility lower when less carbon is present 0.6 - 0.9 Applications Properties Carbon content wt %